The mechanism of bleaching is very complicated and not
completely understood. One opinion is that the color producing agents in
natural fibers are often organic compounds containing conjugated double
bonds. It is known in dye chemistry that conjugation is necessary for an
organic molecule to perform as a dyestuff. Decoloration can occur by breaking
up the chromophore, most likely destroying one or more of the double bonds
within the conjugated system. Oxidative bleaches oxidize color bodies into
For example, double bonds are known to be oxidize into epoxides which
easily hydrolyze into diols. The major bleaching agents used in textile
preparation are sodium hypochlorite, hydrogen peroxide and sodium chlorite.
Other bleaching agents, of lesser importance to textile preparation but
important in consumer laundry products, are perborates, percarbonates and
peracetic acid. All of these are oxidative bleaches. Oxidative bleaches are also
known to degrade cellulose so the objective in bleaching is to optimize
whitening and minimize fiber damage.
MECHANISM OF BLEACHING
Reductive Bleaches reduce color bodies into colorless compounds. Most textile
fibers are bleached with oxidizing bleaches.
MECHANISM OF BLEACHING
Hypochlorite bleaching (OCl-) is the oldest industrial method of bleaching cotton.
Originally, calcium hypochlorite, Ca(OCl)2 was used.
Most cotton fabrics were bleached with sodium hypochlorite up until 1940. Today it
accounts for only 10 % of the cotton bleaching agents in the U.S.
It is however the main stay of home laundry bleaching products. Hypochlorites are
excellent cidal agents for mildew and other bacteria and are used as disinfectants
and to control bacteria in swimming pools.
Sodium hypochlorite is the strongest oxidative bleach -used in textile
processing. Prior to bleaching with hypochlorite, it is necessary to thoroughly scour
fabrics to remove fats, waxes and pectin impurities.
These impurities will deplete the available hypochlorite, reducing its effectiveness for
Sodium hypochlorite is made by bubbling chlorine into a solution of sodium
Conversely, when acid is added to a hypochlorite solution, chlorine gas is
liberated. Product strength of hypochlorites is generally expressed as the
available chlorine content. This relates to the chlorine formed on reaction with
Commercial sodium hypochlorite will have 12 to 15 % active chlorine.
House- hold bleach is 5 % active chlorine. Calcium hypochlorite is sold as a
solid material and contains 65 % active chlorine.
Sodium hypochlorite is the salt of a moderately strong base (OCl-) and a weak
acid (HOCl). Solutions are therefore alkaline. The species present in a solution can be
understood from the following:
Note: Hypochlorous acid (HOCl) is the active bleaching agent.
Effect of pH
pH has a profound effect on bleaching with hypochlorite.
1. If caustic is added to the solution, the equilibrium shifts to the left favoring
the formation of the hypochlorite ion (OC1-) at the expense of hypochlorous
acid (HC1O). Under strongly alkaline conditions (pH > 10), little to no bleaching
2. When acid is added, the equilibrium shifts to the right and the HOCl
concentration increases. At a pH between 5 and 8.5, HOCl is the major specie
present so very rapid bleaching takes place. However, rapid degradation of the
fiber also takes place.
3. When the pH drops below 5, chlorine gas is liberated and the solution has
no bleaching effectiveness at all.
4. The optimum pH for bleaching is between 9 and 10. Although the
concentration of HOCl is small, it is sufficient for controlled bleaching. As HOCl is
used up, the equilibrium conditions continue to replenish it. This pH range is
used to minimize damage to the fiber. Sodium carbonate is used to buffer the
bleach bath to pH 9 to 10.
Effect of Metals
Copper and iron catalyze the oxidation of cellulose by sodium hypochlorite
degrading the fiber. Fabric must be free of rust spots or traces of metals
otherwise the bleach will damage the fabric. Stainless steel equipment is
required and care must be taken that the water supply be free of metal ions
and rust from pipes. Prescouring with chelating agents becomes an important
step when bleaching with hypochlorites.
Fabrics bleached with hypochlorite will develop a distinctive chlorine odor.
This odor can easily be removed with an aftertreatment consisting of sodium
bisulfite and acetic acid.
Effect of Time and Temperature
Time and temperature of bleaching are interrelated. As the temperature
increases, less time is needed. Concentration is also interrelated with time
and temperature. Higher concentrations require less time and temperature. In
practice, one hour at 400 C is satisfactory for effective bleaching.
1. Hypochlorite is used mainly to bleach cellulosic fabrics. It cannot be used
on wool, polyamides (nylon), acrylics or polyurethanes (spandex).
2. These fibers will yellow from the formation of chloramides.
3. Bleaching with hypochlorite is performed in batch equipment.
4. It is not used in continuous operations because chlorine is liberated into
5. Over time, the pad bath decreases in active chlorine causing non-uniform
bleaching from beginning to end of the run.
TYPICAL BATCH PROCEDURE
b. Bleach Cycle:
Hydrogen peroxide was first used to bleach cotton in the 1920's. By 1940, 65
% of all cotton fabrics were bleached with hydrogen peroxide, largely brought about
by the invention of the J-box which lead to continuous processing.
Today, it is estimated that 90 to 95 % of all cotton and cotton/synthetic blends are
bleached with hydrogen peroxide.
It is available commercially as 35, 50 and 70 % solutions.
It is a corrosive, oxidizing agent which may cause combustion when allowed to dry
out on oxidizable organic matter. Decomposition is accelerated by metal
contamination and is accompanied by the liberation of heat and oxygen, which will
support combustion and explosions in confined spaces. The material is an irritant
to the skin and mucous membranes and dangerous to the eyes
Hydrogen peroxide can also decompose. This reaction is catalyzed by metal
ions e.g. Cu++, Fe+++. This reaction is not desired in bleaching because it
is an ineffective use of hydrogen peroxide and causes fiber damage.
Hydrogen peroxide is a weak acid and ionizes in water to form a hydrogen ion and
a perhydroxyl ion. The perhydroxyl ion is the active bleaching agent.
B. Effect of pH
Hydrogen peroxide is an extremely weak acid, Ka = 1.5 X 1012. Since the
perhydroxyl ion is the desired bleaching specie, adding caustic neutralizes the
proton and shifts the reaction to the right. Therefore:
1. at pH < 10, hydrogen peroxide is the major specie so it is inactive as a
2. 2. At pH 10 to 11, there is a moderate concentration of perhydroxyl
ions. pH 10.2 to 10.7 is optimum for controlled bleaching. Sodium
hydroxide is used to obtain the proper pH.
3. 3. At pH > 11, there is a rapid generation of perhydroxyl ions. When the pH
reaches 11.8, all of the hydrogen peroxide is converted to perhydroxyl ions
and bleaching is out of control.
C. Effect of Time and Temperature
Stabilized hydrogen peroxide does not decompose at high temperature therefore
faster and better bleaching occurs at 95 to 100 0C. This feature makes it ideal
for continuous operations using insulated J-boxes or open-width steamers.
Stabilizers must be added to the bleach solution to control the decomposition of hydrogen
peroxide. Stabilizers function by providing buffering action to control the pH at the optimum
level and to complex with trace metals which catalyze the degradation of the fibers.
Stabilizers include sodium silicate, organic compounds and phosphates.
1. Sodium Silicates
Sodium silicates are the most commonly used and most effective hydrogen peroxide bleach
stabilizers. They may be used as colloidal silicate (waterglass), ortho silicate or metasilicate. The
mechanism by which silicate stabilize is not completely
understood, however it is known that silicates have a natural affinity for ferrous ions and ferrous
ions are naturally present in cotton. It is possible that the silicates are adsorbed onto the
ferrous ions in the fiber, producing a species that catalytically enhances bleaching while
reducing bleach decomposition and fiber damage. Stabilization by silicates is enhanced by
the presence of magnesium ions. Magnesium serves as a pH buffer. As the concentration of
OH- rises during bleaching, magnesium hydroxide (Mg(OH)2) precipitates, reducing the
OH- concentration. Bleach solutions containing only magnesium ions have good stability
but the bleaching effectiveness is not as good as when silicates are included. Silicates as
stabilizers have one drawback, they tend to polymerize and form insoluble silicates. They
becomes hard deposits which build-up in the machines causing the fabric to be abraded.
Also some of the deposits will form in the cloth, giving it a harsh, raspy hand, a real negative for
2. Organic Stabilizers
Organic stabilizers avoid the problems associated with sodium silicates. These products are
often referred to as silicate free or non-silicate stabilizers. They may be based on
sequestering agents, protein degradation products or certain surfactants. The commercial
products are of two types, those designed only to be stabilizers and those which combine
stabilization with other properties such as detergency and softening. For some
bleaching methods, organic stabilizers may be used alone, while in others, they are best
used in combination with silicates.
Tetrasodium pyrophosphate (TSPP) and hexametaphosphates are of interest as stabilizers
in alkaline bleach baths under the following conditions:
1. The alkalinity of the bleach must not be higher than pH 10 since above
this, the stabilizing effect decreases rapidly.
2. Temperature of the bleach bath is limited to 60 0 C. Higher temperatures reduce
stabilizing properties. They should be used with ammonia, not caustic soda or soda
3. TSPP at high pH and temperature is converted to trisodium phosphate which has little
stabilizing effect. The use of TSPP is limited to bleaching wool and silk which are
sensitive to high pH and high temperatures. As opposed to
silicates, pyrophosphates are precipitated from solution in the presence of
calcium and magnesium and therefore do not develop full stabilizing power.
Hydrogen peroxide is the bleach most widely used for cellulosic fibers [cotton,
flax, linen, jute etc.) and well as wool, silk, nylon and acrylics. Unlike
hypochlorites, peroxide bleaching does not require a full scour.
Residual fats, oils, waxes and pectines do not reduce the bleaching
effectiveness of hydrogen peroxide. Additionally it can be used on continuous
equipment. Since it ultimately decomposes to oxygen and water, it doesn't
create effluent problems.
Typical Bleaching Procedures
a. Bath Formulation
1. Hydrogen peroxide (35 %)
2. Wetting agent
4. Sodium silicate
5. Magnesium sulfate (Epsom's salt)
b. Bleach Cycle
1. Run 60 to 90 minutes at 95 to 1000 C.
2. Drop bath
a. Bath Formulation
Double above formulation
b. Bleach Cycle
1. Saturate goods to 100 % wet pick up
2. Steam in J -box or steamer for one hour
3. Wash thoroughly
1. Among the oxidizing bleaching agents, only hydrogen peroxide provides a high
bleaching effect at reasonable costs, especially if modern short-term
bleaching processes are used with only a few minutes bleaching time.
2. Peroxide bleaching keeps the fibre quality intact.
3. Cotton can be bleached with peroxide in a single stage. Other processes
require two or three bleaching stages,(desize with scour, scour with bleach
and desize with scour and bleach).
4. No separate pre treatment is necessary because hot, alkaline bleaching has
not only a bleaching but also a cleaning effect, it therefore combines the
advantages of an alkaline extraction with the bleaching treatment.
5. Animal fibres can only be bleached with peroxide to a high and stable degree
- Corrosion of stainless steel equipment does not occur during peroxide
6. The spent peroxide baths still contain residuals of hydrogen peroxide which
fever the degradation of the organic impurities in the effluent, and this helps
to decrease the chemical oxygen demand (COD).
Advantages of Peroxide Bleaching:
Bleaching with sodium chlorite is carried out under acidic conditions which
releases chlorine dioxide, a toxic and corrosive yellow-brown gas. Sodium chlorite
is sold as an 80% free flowing powder. Chlorine dioxide is thought to be the
active bleaching specie.
It is not used much in the USA for bleaching but it is sometimes used to strip
dyed goods and is often described as the bleach of last resort.
One advantage of sodium chlorite bleaching is that it leaves the fabrics with a
soft hand. Because of the gaseous nature, toxicity and corrosiveness of chlorine
dioxide, special attention must be paid to the equipment. It must be designed so as
to not allow the gas to escape into the work place. Emissions into the atmosphere
are of concern too. The gas corrodes even stainless steel so special passivating
treatments must be carried out to prolong the life of the equipment.
When a solution of sodium chlorite is acidified, chlorine dioxide (ClO2),
hypochlorous acid (HClO2), sodium chlorate (NaC1O3) and sodium chloride are
formed. Chlorine dioxide and hypochlorous acid are bleaching species, sodium
chlorate and sodium chloride are not. The reactions may be written:
A. Effect of pH
Chlorine dioxide is favored at low pH - 1 to 2.5. It is a more active bleaching
agent than hypochlorous acid which is favored at pH 4 to 5. However
chlorine dioxide is a corrosive and toxic gas. When generated too rapidly, it
escapes from the bleaching bath into the atmosphere creating an explosion and
health hazard. Once the chlorine dioxide is out of solution, its effectiveness as a
bleach is lost.
B. Bleaching Mechanism
Chlorine dioxide only reacts with aldehyde groups without affecting hydroxyls or
glucosidic linkages. Aldehydes are converted to carboxylic acids. This is of
practical importance because cellulose is very slightly damaged, even when
high degree of whiteness is obtained. When strong acids are used, the low pH
will damage the fiber at the glucosidic linkage so buffers like sodium dihydrogen
orthophosphate are commonly used. Sodium acetate and the other sodium
phosphate salts are also effective buffers. The acid is added incrementally over
the bleach cycle, not all at once. This too controls the bath pH and avoids rapid
evolution of chlorine dioxide.
C. Effect of Temperature
Little or no bleaching takes place at temperatures below 50C, however the
bleaching rate increases considerably up to 90C. Going to the boil is not
recommended because it leads to excessive loss of chlorine dioxide with the
Ammonium, potassium and sodium persulfates are oxidizing agent that find use
in textile processing. They are used to:
1. bleach protein fibers in combination with hydrogen peroxide,
2. activate cold bleaching of cellulosics with sodium chlorite,
3. oxidize vat and sulfur dyes, and
4. bleach fur and skins in combination with hydrogen peroxide.
B. Perborates and Percarbonates
Both perborates and percarbonates are used when full whites are not necessary such
as for improving the ground color when dyeing light or pastel shades. They are often
found as solid bleaches in home laundry products when fabric care require mild
C. Peracetic Acid
Peracetic acid as a textile bleach is used mainly in bleaching nylon and acetate.
Some other oxidative bleaches are persulfates, perborates,
percarbonates and peracetic acid.
Reductive bleaches work by reducing colored impurities into colorless
forms. Reductive bleaches can be generalized as compounds which supply
hydrogen for hydrogenating or reducing color bodies. For
example, aldehydes are reduced to alcohols by the addition of one mole of
hydrogen, double bonds are saturated by the addition of one mole of hydrogen.
Both reactions can account for the decoloration of color bodies by breaking up
A. Sulfur Dioxide
In the early days (prior to 1940), sulfur dioxide was used to bleach wool.
Moistened fabrics were hung on poles in a sealed chamber (called a stove). A pot
of sulfur was ignited and the goods exposed overnight to the sulfur dioxide
vapors. The bleached goods were rinsed in water containing sodium sulfite
which removed the retained sulfur dioxide by forming sodium bisulfite. A
disadvantage of this method of bleaching wool was that the white was not
permanent when exposed to sun and air.
B. Sodium Dithionate (Sodium Hydrosulfite)
Sodium hydrosulfite, better known as "hydro" finds major usage as a reducing agent in
textile processing. One of its main use is to reduce vat and sulfur dyes into the water
soluble leuco form. As such it can be used to strip dyed goods, ergo bleach dyed
goods. In water and with heat, hydro is oxidized into sodium bisulfite, liberating
hydrogen - the reducing agent.
Hydro can also be used to bleach wool. It's not used much because it tends to
impart a harsh handle. Reducing agents also are known to break cystine crosslinks
in protein fibers. When the crosslinks are reformed by oxidation (oxygen in air or
hydrogen peroxide) the protein fiber can be given a " permanent set". This has
been used as a finishing treatment to impart durable creases to wool fabrics and to
impart permanent waves to human hair.
AATCC Test Method 82, Fluidity of Dispersions of Cellulose from Bleached Cotton Cloth
AATCC Test Method 110, Reflectance, Blue and Whiteness of Bleached Fabrics are the
main tests used to determine the effectiveness of bleaching
Since yellow impurities adsorb blue light, AATCC Test Method 110 measures the
amount of blue light reflected by the goods, against a white standard (usually a
ceramic tile). This gives a measure of how well the yellow impurities were
removed by bleaching. Whiteness is measured by reflectance of green light and
by the removal of yellow impurities.
The equation below is used to calculate whiteness. The standard ceramic tile
is measured and set to equal 100. The other specimen are rated against this
standard. Unbleached fabrics will give values in the 50 to 60 range. Well
breached fabrics will rank 95 or better.
W = whiteness
B = blue reflectance
G = green reflectance
The theory behind fluidity measurements is that damaged cellulose has a lower
69molecular weight than undamaged cellulose. Solutions from undamaged fibers are
less fluid than those from damaged fibers. Fluidity is measured by dissolving cotton in
cupriethylene diamine and determining the solutions's viscosity. Viscosity of
polymer solutions is directly related to the polymer's molecular weight so a fluidity
measurement, in reality, is a viscosity measurement. The difference between
viscosity and fluidity is the units used to express the results. Viscosity
measurements use water as the reference standard, setting it equal to 1 centipoise.
Therefore the higher the polymer molecular weight, the higher the viscosity number.
The fluidity scale (Rhes) is just the opposite of the viscosity scale. Low numbers are
used to describe high viscosity solutions while high numbers describe low viscosity
(more fluid) ones. Undamaged cellulose will have low fluidity numbers and damaged
cellulose will have high ones.
1. Full 1/3 Viscometer with cupramonium solution
2. Put 0.5 gm oxycellulose to the solution & put stainless steel into viscometer
3. Full viscometer is filled with cupraamonium solution
4. When top rubber stopper close up then this solution goes up into the capillary
& no air is in the capillary.
5. Viscometer is covered with black fabric to protect from sunlight
6. The viscometer keep rotate at 4 r.p.m onto wheel until cellulose dissolve into
7. The viscometer keep rotating for whole night at 20⁰ C.
1. Open the upper & lower stopper
then the solution goes round into
2. Calculate the time to pass the
solution from upper measuring
mark to lower measuring mark.
Damage in Bleaching:
Cellulose may be easily oxidized into a variety of product known as oxycellulose.
Now-a-days, scouring & bleaching is combination process. Formulation of
oxycellulose causes strength loss. There are three points at which oxidizing agents
can attack the glucose molecule.
Estimation of Damage:
Physically: By testing strength before & after bleaching
a) Fluidity Test,
b) Copper Number,
c) Methylene Blue Test.
Damage in Bleaching
BEN-BLEACH Continuous Desizing – Scouring - Bleaching Range
Cross section of whole Range
Different Sections of range
INJECTA for desizing
EXTRACTA for washing
IMPACTA for impregnating
REACTA a combination steamer with tight strand fabric guidance and roller bed plaiting
FORTRACTA for pre-washing
EXTRACTA/TRIKOFLEX for washing